Polymer Melt Rheology. Introduction to Viscoelastic Behavior. TimeTemperature Equivalence


 Merryl McBride
 3 years ago
 Views:
Transcription
1 Topics to be Covered Polymer Melt Rheology Introduction to Viscoelastic Behavior TimeTemperature Equivalence Chapter 11 in CD (Polymer Science and Engineering)
2 Polymer Melt Rheology
3 δ τ xy Newton s Law z θ v 0 The most convenient way to describe deformation under shear is in terms of the angle θ through which the material is deformed; tanθ = δ z = γ xy Then if you shear a fluid at a constant rate γ xy δ = z = v 0 z dx dz γ xy = dv dz = d dt y Just as stress is proportional to strain in Hooke s law for a solid, the shear stress is proportional to the rate of τ xy γ strain for a fluid xy τ xy = η γ xy
4 Newtonian and Non  Newtonian Fluids Shear Stress.. τ xy = η a (γ) γ Slope = η a Shear Thinning Newtonian Fluid (η = slope) Shear Thickening Strain Rate When the chips are down, what do you use?
5 Variation of Melt Viscosity with Strain Rate Log η a (Pa) Zero Shear Rate Viscosity Log γ (sec 1 ) SHEAR RATES ENCOUNTERED IN PROCESSING Compression Molding Calendering Extrusion Injection Molding Spin Drawing Strain Rate (sec 1 )
6 How Do Chains Move  Reptation D ~ 1/M 2 η 0 ~ M 3
7 Variation of Melt Viscosity with Molecular Weight Log η m + constant Poly(dimethylsiloxane) Poly(isobutylene) Poly(ethylene) Poly(butadiene) Poly(tetramethyl psilphenyl siloxane) Poly(methyl methacrylate) Poly(ethylene glycol) Poly(vinyl acetate) Poly(styrene) η m = K L (DP) 1.0 η m = K H (DP) 3.4 Redrawn from the data of G. C. Berry and T. G. Fox, Adv. Polym. Sci., 5, 261 (1968) Log M + constant 5
8 Entanglements Short chains don t entangle but long ones do  think of the difference between a nice linguini and spaghettios, the little round things you can get out of a tin (we have some value judgements concerning the relative merits of these two forms of pasta, but on the advice of our lawyers we shall refrain from comment).
9 Entanglements Viscosity  a measure of the frictional forces acting on a molecule η m = K L (DP) 1.0 Small molecules  the viscosity varies directly with size At a critical chain length chains start to become tangled up with one another, however Then η m = K H (DP) 3.4
10 Entanglements and the Elastic Properties of Polymer Melts d 0 d d/d C 180 C Depending upon the rate at which chains disentangle relative to the rate at which they stretch out, there is an elastic component to the behavior of polymer melts. There are various consequences as a result of this C Strain Rate at Wall (sec 1 ) Jet Swelling
11 Melt Fracture Reproduced with permission from J. J. Benbow, R. N. Browne and E. R. Howells, Coll. Intern. Rheol., Paris, JuneJuly 1960.
12 Viscoelasticity If we stretch a crystalline solid, The energy is stored in the Chemical bonds If we apply a shear stress to A fluid,energy is dissipated In flow VISCOELASTIC Ideally elastic behaviour Ideally viscous behaviour
13 Viscoelasticity Homer knew that the first thing To do on getting your chariot out in the morning was to put the wheels back in. (Telemachus,in The Odyssey, would tip his chariot against a wall) Robin hood knew never to leave his bow strung
14 Experimental Observations Creep Stress Relaxation Dynamic Mechanical Analysis
15 Creep and Stress Relaxation 5lb 5lb 5lb 5lb Creep  deformation under a constant load as a function of time TIME Stress Relaxation  constant deformation experiment 5lb 4lb 3lb 2lb TIME
16 Creep(%) Redrawn from the data of W. N. Findley, Modern Plastics, 19, 71 (August 1942) 2695psi 2505 psi 2305 psi 2008 psi Creep and Recovery 30 Strain (c) VISCOELASTIC RESPONSE Creep psi Stress applied Stress removed Recovery } deformation Permanent Time psi 1018 psi Time (hours) 8000
17 Strain vs. Time Plots  Creep (a) PURELY ELASTIC RESPONSE Strain (b) PURELY VISCOUS RESPONSE Strain Stress applied Stress removed Time Shear Stress applied Shear Stress removed Permanent Deformation Time Strain (c) VISCOELASTIC RESPONSE Creep Stress applied Stress removed Recovery } Permanent deformation Time
18 Stress Relaxation 10 Redrawn from the data of J.R. McLoughlin and A.V. Tobolsky. J. Colloid Sci., 7, 555 (1952) C 60 0 C The data are not usually reported as a stress/time plot, but as a modulus/time plot. This time dependent modulus, called the relaxation modulus, is simply the time dependent stress divided by the (constant) strain E(t ) = σ (t ) ε 0 Log E(t), (dynes/cm 2 ) C 92 0 C C 80 0 C C Stress relaxation of PMMA C C C C Time (hours)
19 Amorphous Polymers  Range of Viscoelastic Behaviour V s Rubbery Semi Solid Liquid Like Hard Glass Leather Soft Like Glass T T g
20 Viscoelastic Properties 0f Amorphous Polymers Log E (Pa) 10 Glassy Region Rubbery Plateau Low Molecular Weight Temperature Crosslinked Elastomers Melt Measured over Some arbitrary Time period  say 10 secs
21 Viscoelastic Properties 0f Amorphous Polymers Stretch sample an arbitrary amount, measure the stress required to maintain this strain. Then E(t) = σ(t)/ε Log E(t) (dynes/cm 2 ) Low Molecular Weight Glassy Region Glass Transition Rubbery Plateau High Molecular Weight Log Time (Sec)
22 Time Temperature Equivalence Log E(t) (dynes/cm 2 ) Low Molecular Weight Glassy Region Glass Transition Rubbery Plateau High Molecular Weight Log E (Pa) Log Time (Sec) 6 Rubbery Plateau Glassy Region Low Molecular Weight Temperature Crosslinked Elastomers Melt
23 Relaxation in Polymers First consider a hypothetical isolated chain in space,then imagine stretching this chain instantaneously so that there is a new end  to  end distance.the distribution of bond angles (trans, gauche, etc) changes to accommodate the conformations that are allowed by the new constraints on the ends. Because it takes time for bond rotations to occur, particularly when we also add in the viscous forces due to neighbors, we say the chain RELAXES to the new state and the relaxation is described by a characteristic time τ. How quickly can I do these things?
24 Amorphous Polymers  the Four Regions of Viscoelastic Behavior Log E (Pa) Low Molecular Weight Polymer Melt Temperature GLASSY STATE  conformational changes severely inhibited. Tg REGION  cooperative motions of segments now occur,but the motions are sluggish ( a maximum in tan δ curves are observed in DMA experiments) RUBBERY PLATEAU  τ t becomes shorter,but still longer than the time scale for disentanglement TERMINAL FLOW  the time scale for disentanglement becomes shorter and the melt becomes more fluid like in its behavior
25 Semicrystalline Polymers Motion in the amorphous domains constrained by crystallites α Motions above Tg are often more complex,often involving coupled processes in the crystalline and amorphous domains γ β LDPE LPE Less easy to generalize  polymers often have to be considered individually  see DMA data opposite Redrawn from the data of H. A. Flocke, Kolloid Z. Z. Polym., 180, 188 (1962).
26 Topics to be Covered Simple models of Viscoelastic Behavior TimeTemperature Superposition Principle Chapter 11 in CD (Polymer Science and Engineering)
27 Mechanical and Theoretical Models of Viscoelastic Behavior GOAL  relate G(t) and J(t) to relaxation behavior. We will only consider LINEAR MODELS. (i.e. if we double G(t) [or σ(t)], then γ(t) [or ε(t)] also increases by a factor of 2 (small loads and strains)). TENSILE EXPERIMENT Stress Relaxation Creep E(t ) = σ(t) ε 0 D(t) = ε(t) σ 0 Linear Time Independent Behavior E = 1 D Time Dependent Behavior E(t ) 1 D(t) SHEAR EXPERIMENT G(t) = τ(t) γ 0 J(t) = γ (t) τ 0 G = 1 J G(t) 1 J(t)
28 Simple Models of the Viscoelastic Behavior of Amorphous Polymers Keep in mind that simple creep and recovery data for viscoelastic materials looks something like this Strain (c) VISCOELASTIC RESPONSE Creep Stress applied Stress removed Recovery } Permanent deformation Time
29 Simple Models of the Viscoelastic Behavior of Amorphous Polymers While stress relaxation data look something like this; Log E(t) (dynes/cm 2 ) Low Molecular Weight Glassy Region Glass Transition Rubbery Plateau High Molecular Weight Log Time (Sec)
30 Simple Models of the Viscoelastic Behavior of Amorphous Polymers Extension l 0 Hooke's law σ = Eε l σ I represent linear elastic behavior σ = Eε
31 Simple Models of the Viscoelastic Behavior of Amorphous Polymers Viscous flow v 0 y v Newtonian fluid. τ = ηγ xy σ = η dε dt
32 Strain v s. Time for Simple Models PURELY ELASTIC RESPONSE Strain σ = Eε PURELY VISCOUS RESPONSE σ = η dε dt Strain Stress applied Stress removed Time Permanent Deformation Shear Stress applied Shear Stress removed Time
33 Maxwell Model Maxwell was interested in creep and stress relaxation and developed a differential equation to describe these properties Maxwell started with Hooke s law σ = Eε _dσ dt Then allowed σ to vary with time = Ε _dε dt Writing for a Newtonian fluid σ = η _dε dt Then assuming that the rate of strain is simply a sum of these two contributions _dε dt = _σ η + _1 _dσ Ε dt
34 MAXWELL MODEL  Creep and Recovery Strain Creep and recovery _dε dt = _σ η 0 t Time Strain Recall that real viscoelastic behaviour looks something like this A picture representation of Maxwell s equation 0 t Time
35 Maxwell Model Stress Relaxation _dε dt = _dε dt _σ η = + 0 _1 _dσ Ε dt In a stress relaxation experiment Hence Where dσ _ σ = _σ η dt σ = σ 0 exp[t/τ ] t τ t = _η Ε Relaxation time Log (E r /E 0 ) Log (t/τ )
36 Maxwell Model Stress Relaxation Log E(t) (Pa) The Maxwell model gives curves like this, OR like this Real data looks like this MAXWELL MODEL E(t ) = σ (t) ε 0 = σ 0 ε 0 exp t τ t Time
37 Voigt Model Maxwell model essentially assumes a uniform distribution Of stress.now assume uniform distribution of strain  VOIGT MODEL Picture representation Equation σ(t) = Eε(t) + η dε(t) dt (Strain in both elements of the model is the same and the total stress is the sum of the two contributions) σ 1 σ 2 σ = σ 1 + σ 2
38 Voigt Model  Creep and Stress Relaxation Strain σ 1 σ 2 σ = σ 1 + σ 2 Gives a retarded elastic response but does not allow for ideal stress relaxation,in that the model cannot be instantaneously deformed to a given strain. But in CREEP σ = constant, σ 0 σ(t) = σ 0 = Eε(t) + η dε(t) ε(t) dt + τ t Strain = _ σ η 0 dε(t) dt RETARDED ELASTIC RESPONSE σ ε(t) = _ [1 exp (t/τ )] Ε 0 τ t  retardation time (η/e) t t 1 t 2 Time
39 Summary What do the strain/time plots look like?
40 Problems with Simple Models I can t t do creep And I can t t do stress relaxation The maxwell model cannot account for a retarded elastic response The voigt model does not describe stress relaxation Both models are characterized by single relaxation times  a spectrum of relaxation times would provide a better description NEXT  CONSIDER THE FIRST TWO PROBLEMS THEN THE PROBLEM OF A SPECTRUM OF RELAXATION TIMES
41 Four  Parameter Model Elastic + viscous flow + retarded elastic E M Eg CREEP ε σ_ σ 0 t σ = + η + _ [1 exp (t/τ )] M Ε 0 M Ε 0 M t E V η V Strain Retarded or Anelastic Response Stress applied Elastic Response Stress removed } Permanent deformation Time η M
42 Distributions of Relaxation and Retardation Times We have mentioned that although the Maxwell and Voigt models are seriously flawed, the equations have the right form. What we mean by that is shown opposite, where equations describing the Maxwell model for stress relaxation and the Voigt model for creep are compared to equations that account for a continuous range of relaxation times. E(t ) = Stress Relaxation E(t ) = 0 E(τ t )exp( t/τ t )dτ t D(t) = D( τ t )1 [ exp( t/ τ t )] d 0 E 0 exp ( t / τ t ) Creep D(t) = D 0 [ 1 exp( t/ )] τ t τ t These equations can be obtained by assuming that relaxation occurs at a rate that is linearly proportional to the distance from equilibrium and use of the Boltzmann superposition principle. We will show how the same equations are obtained from models.
43 The Maxwell  Wiechert Model _dε dt = _σ η = _σ η = _σ η + _1 _dσ Ε dt + _1 _dσ Ε dt + _1 _dσ Ε dt E 1 E 2 E 3 Consider stress relaxation 0 _dε dt = 0 σ = σ exp[t/τ ] 1 0 t1 σ = σ exp[t/τ ] 2 0 t2 σ = σ exp[t/τ ] 3 t3 η 1 η 2 η 3
44 Distributions of Relaxation and Retardation Times Stress relaxation modulus E(t) = σ(t)/ε 0 σ(t) = σ + σ + σ E(t) = σ exp (t/τ 01 ) + σ exp (t/τ 02 ) + σ exp (t/τ 03) ε 01 0 Or, in general ε 02 0 E(t) = Σ E n exp (t/τ tn ) where E = n ε 03 0 σ ε 0n 0 Similarly, for creep compliance combine voigt elements to obtain D(t) =ΣD n [1 exp (t/τ tn )]
45 Log E(t) (dynes/cm 2 ) Distributions of Relaxation and Retardation Times Example  the Maxwell  Wiechert Model With n = Glassy Region Glass Transition Rubbery Plateau Melt Log Time (Sec) Log E(t) (Pa) Log time (min) E(t) = Σ E n exp (t/τ tn ) n = 2 4
46 Time  Temperature Superposition Principle Log E(t) (dynes/cm 2 ) Recall that we have seen that there is a time  temperature equivalence in behavior Log E (Pa) 10 9 Glassy Region 6 Glass 10 Transition 5 9 Rubbery 4 8 Plateau Low Molecular High 5 Weight Molecular Weight Log Time (Sec) 8 7 Rubbery Plateau Glassy Region Low Molecular Weight Temperature Crosslinked Elastomers Melt This can be expressed formally in terms of a superposition principle
47 Time Temperature Superposition Principle  Creep T 3 > T 2 > T 1 ε(t) T σ0 G' T 3 T 2 T 1 log t Master Curve at T 0 0 C ε(t) T σ0 log a T 0 T 0 [log t  log a T ] T
48 Stress Relaxation Modulus dynes/cm 2 Time Temperature Superposition Principle  Stress Relaxation Stress Relaxation Data C C C C C C C C 0.0 C +25 C +50 C Log Shift Factor Master Curve at 25 0 C SHIFT FACTOR vs TEMPERATURE Temperature 0 C Time (hours)
49 Relaxation Processes above T g  the WLF Equation From empirical observation Log a = C (T  T ) 1 s For Tg > T < ~(Tg C) T C + (T  T ) 2 s Originally thought that C 1 and C 2 were universal constants, = and 51.6, respectively,when T s = Tg. Now known that these vary from polymer to polymer. Homework problem  show how the WLF equation can be obtained from the relationship of viscosity to free volume as expressed in the Doolittle equation
50 Semi  Crystalline Polymers NON  LINEAR RESPONSE TO STRESS.SIMPLE MODELS AND THE TIME  TEMPERATURE SUPERPOSITION PRINCIPLE DO NOT APPLY Temperature Tm Tg Amorphous melt Rigid crystalline domains Rubbery amorphous domains Rigid crystalline domains Glassy amorphous domains
HW 10. = 3.3 GPa (483,000 psi)
HW 10 Problem 15.1 Elastic modulus and tensile strength of poly(methyl methacrylate) at room temperature [20 C (68 F)]. Compare these with the corresponding values in Table 15.1. Figure 15.3 is accurate;
More informationNotes on Polymer Rheology Outline
1 Why is rheology important? Examples of its importance Summary of important variables Description of the flow equations Flow regimes  laminar vs. turbulent  Reynolds number  definition of viscosity
More informationLong term performance of polymers
1.0 Introduction Long term performance of polymers Polymer materials exhibit time dependent behavior. The stress and strain induced when a load is applied are a function of time. In the most general form
More information3 rd Year Dental Materials Science
3 rd Year Dental Materials Science Dr. Graham Cross School of Physics and CRANN SFI Nanoscience Building, Rm 1.5 http://www.tcd.ie/physics/people/graham.cross/ Graham.Cross@tcd.ie 16.11.2007 Dental Materials
More informationOversimplified Viscoelasticity
THE MAXWELL MODEL At time t = 0, suddenly deform to constant displacement X o. The force F is the same in the spring and the dashpot. F = K e X e = K v (dx v /dt) (120) X e is the displacement of the
More informationStress Strain Behavior (I) Stress Strain Behavior (II) Stress Strain Behavior (III)
Chapter Outline: Characteristics, Applications, and Processing of Polymers Mechanical properties StressStrain Behavior Deformation of Semicrystalline Polymers Crystallization, Melting, Glass Transition
More informationM n = (DP)m = (25,000)(104.14 g/mol) = 2.60! 10 6 g/mol
14.4 (a) Compute the repeat unit molecular weight of polystyrene. (b) Compute the numberaverage molecular weight for a polystyrene for which the degree of polymerization is 25,000. (a) The repeat unit
More informationRheology and Polymer Characterization
Rheology and Polymer Characterization Asst Prof Anongnat Somwangthanaroj Anongnat.s@chula.ac.th 20 Sep 2010 http://pioneer.netserv.chula.ac.th/~sanongn1/course.html Fundamentals: Why Rheology? Fundamental
More informationRheological Properties of Topical Formulations
Rheological Properties of Topical Formulations Hemi Nae, PhD Hydan Technologies, Inc. Key Words Complex Modulus, Creep/Recovery, Dilatant Flow, Dynamic Viscosity, Flow, Flow Curve, Flow Models, Frequency
More information3.3. Rheological Behavior of Vinyl Ester Resins
3.3. Rheological Behavior of Vinyl Ester Resins 3.3.1. Introduction Rheology is the study of the deformation and flow of matter 1. There has been significant appreciation of the importance of the rheological
More informationRheology of polymer systems/ Reologia dos sistemas poliméricos
Rheology of polymer systems/ Reologia dos sistemas poliméricos 1. Viscosity/Viscosidade Jorge Morgado, IST Polymers Molecular materials in nature COMPLEX behaviour Viscosity of concentrated solu1ons and
More informationViscoelasticity of Polymer Fluids.
Viscoelasticity of Polymer Fluids. Main Properties of Polymer Fluids. Entangled polymer fluids are polymer melts and concentrated or semidilute (above the concentration c) solutions. In these systems polymer
More informationElastic Properties of Polymer Melts Filled with Nanoparticles
Elastic Properties of Polymer Melts Filled with Nanoparticles Helmut Münstedt and Christian Triebel Citation: AIP Conf. Proc. 1375, 21 (211); doi: 1.163/1.364479 View online: http://dx.doi.org/1.163/1.364479
More informationStress Relaxation Study of Paper and Plastic Film based Packaging Material
Master's Degree Thesis ISRN: BTHAMTEX2009/D02SE Stress Relaxation Study of Paper and Plastic Film based Packaging Material Rajdip Roy Lu Qi Department of Mechanical Engineering Blekinge Institute
More informationσ = F / A o Chapter Outline Introduction Mechanical Properties of Metals How do metals respond to external loads?
Mechanical Properties of Metals How do metals respond to external loads? and Tension Compression Shear Torsion Elastic deformation Chapter Outline Introduction To understand and describe how materials
More informationKMχ /γ = (1.3E 23 )(88.2)(3.4138 E 20 ) 3.05 = 0.12834. T g = (302)*( 0.12834 / (10.12834) ) = 44.5 o K
Problem Set #5 Solutions Chemical ngineering 60/60 Problem 8.4 We re given T g as 0 o C and given the viscosity at 5 o C, and asked to find the viscosity at 40 o C. We can use equation 8.48 (WLF equation).
More informationPolymer Analysis with MCR Rheometers. MCR Series
Polymer Analysis with MCR Rheometers MCR Series Polymer Analysis Today, polymers are among the most important materials in existence as the properties of polymers can be adapted in a very wide range to
More information1. Fluids Mechanics and Fluid Properties. 1.1 Objectives of this section. 1.2 Fluids
1. Fluids Mechanics and Fluid Properties What is fluid mechanics? As its name suggests it is the branch of applied mechanics concerned with the statics and dynamics of fluids  both liquids and gases.
More informationThermoplastic Material Testing for Use in Sigmasoft
Thermoplastic Material Testing for Use in Sigmasoft + technical center for materials a DatapointLabs affiliate Materials Testing Data Infrastructure Productivity Software Plastic Rubber Film Metal Foam
More informationChapter Outline. Mechanical Properties of Metals How do metals respond to external loads?
Mechanical Properties of Metals How do metals respond to external loads? Stress and Strain Tension Compression Shear Torsion Elastic deformation Plastic Deformation Yield Strength Tensile Strength Ductility
More informationLOW TEMPERATURE TESTING OF ELASTOMERS
LOW TEMPERATURE TESTING OF ELASTOMERS Presented at the Spring Technical Meeting of the New York Rubber Group Thursday, March 25, 1999 By, Andrew C. Farinella and Daniel L. Hertz, Jr. LOW TEMPERATURE DATA
More informationA Beginner s Guide DMA
FREQUENTLY ASKED QUESTIONS Dynamic Mechanical Analysis (DMA) A Beginner s Guide This booklet provides an introduction to the concepts of Dynamic Mechanical Analysis (DMA). It is written for the materials
More informationLecture 4.1: Thermoplastics and Thermosets
Lecture 4.1: Thermoplastics and Thermosets The word plastic comes from the Greek word Plastikos, meaning able to be shaped and molded. Plastics can be broadly classified into two major groups on the basis
More informationChapter Outline. Mechanical Properties of Metals How do metals respond to external loads?
Mechanical Properties of Metals How do metals respond to external loads? Stress and Strain Tension Compression Shear Torsion Elastic deformation Plastic Deformation Yield Strength Tensile Strength Ductility
More information4 Thermomechanical Analysis (TMA)
172 4 Thermomechanical Analysis 4 Thermomechanical Analysis (TMA) 4.1 Principles of TMA 4.1.1 Introduction A dilatometer is used to determine the linear thermal expansion of a solid as a function of temperature.
More informationNonNewtonian Flows. R. Shankar Subramanian Department of Chemical and Biomolecular Engineering Clarkson University. τ = ηθ
NonNewtonian Flows R. Shankar Subramanian Department of Chemical and Biomolecular Engineering Clarkson University Fluids such as water, air, ethanol, and benzene are Newtonian. This means that a plot
More informationStrain and deformation
Outline Strain and deformation a global overview Mark van Kraaij Seminar on Continuum Mechanics Outline Continuum mechanics Continuum mechanics Continuum mechanics is a branch of mechanics concerned with
More informationInjection Molding. Materials. Plastics 2.008. Outline. Polymer. Equipment and process steps. Considerations for process parameters
Outline 2.008 Polymer Equipment and process steps Injection Molding Considerations for process parameters Design for manufacturing, tooling and defects 1 2.008 spring 2004 S. Kim 2 Materials Solid materials
More informationThermoplastic composites
Thermoplastic composites Definition By definition, a thermoplastic is a material based on polymer (macromolecular compound) which can be shaped, in a liquid (viscous) state at a temperature either higher
More informationFluids and Solids: Fundamentals
Fluids and Solids: Fundamentals We normally recognize three states of matter: solid; liquid and gas. However, liquid and gas are both fluids: in contrast to solids they lack the ability to resist deformation.
More informationPolymers: Introduction
Chapter Outline: Polymer Structures Hydrocarbon and Polymer Molecules Chemistry of Polymer Molecules Molecular Weight and Shape Molecular Structure and Configurations Copolymers Polymer Crystals Optional
More informationPraktikum III. Experiment P4. Simulation of Polymer Behavior in Step Shear Rate Flow using the Reptation Model
Praktikum III Fall Term 211 Experiment P4 Simulation of Polymer Behavior in Step Shear Rate Flow using the Reptation Model A lab report written by: Baumli Philipp baumlip@student.ethz.ch Date of the experiment:
More informationModern Construction Materials Prof. Ravindra Gettu Department of Civil Engineering Indian Institute of Technology, Madras
Modern Construction Materials Prof. Ravindra Gettu Department of Civil Engineering Indian Institute of Technology, Madras Module  2 Lecture  2 Part 2 of 2 Review of Atomic Bonding II We will continue
More information4 The strength of the lithosphere
4 The strength of the lithosphere Constitutive equations specify the relations between stress and strain or the time derivatives of strain and thus can be used in conjunction with the equations of motion
More informationLow Temperature Properties of Polymers
TECHNICAL WHITEPAPER Low Temperature Properties of Polymers Introduction Most plastics at room temperature show their familiar properties of flexibility (a low Young s modulus) and high resistance to cracking
More informationA8 Thermal properties of materials
A8 Thermal properties of materials Thermal properties the melting temperature, T m, and the glass temperature (temperatura de transição vítrea), T g, relate directly to the strength of the bonds in the
More informationCHAPTER 6 MECHANICAL PROPERTIES OF METALS PROBLEM SOLUTIONS
CHAPTER 6 MECHANICAL PROPERTIES OF METALS PROBLEM SOLUTIONS Concepts of Stress and Strain 6.1 Using mechanics of materials principles (i.e., equations of mechanical equilibrium applied to a freebody diagram),
More informationYield Criteria for Ductile Materials and Fracture Mechanics of Brittle Materials. τ xy 2σ y. σ x 3. τ yz 2σ z 3. ) 2 + ( σ 3. σ 3
Yield Criteria for Ductile Materials and Fracture Mechanics of Brittle Materials Brittle materials are materials that display Hookean behavior (linear relationship between stress and strain) and which
More information15.32 Of those polymers listed in Table 15.2, which polymer(s) would be best suited for use as ice cube trays? Why?
15.31 Name the following polymer(s) that would be suitable for the fabrication of cups to contain hot coffee: polyethylene, polypropylene, poly(vinyl chloride), PET polyester, and polycarbonate. Why? This
More informationDeveloping an ANSYS Creep Model for Polypropylene from Experimental Data
Developing an ANSYS Creep Model for Polypropylene from Experimental Data Abstract Martin J. Dropik David H. Johnson, P.E. David E. Roth, P.E. Penn StateErie, Erie, PA, USA This paper describes a procedure
More informationMaterial Science. Prof. Satish V. Kailas Associate Professor Dept. of Mechanical Engineering, Indian Institute of Science, Bangalore India
Material Science Prof. Satish V. Kailas Associate Professor Dept. of Mechanical Engineering, Indian Institute of Science, Bangalore 5612 India Chapter 15. Thermal properties Engineering materials are important
More informationTA INSTRUMENTS DYNAMIC MECHANICAL ANALYZER
TA INSTRUMENTS DYNAMIC MECHANICAL ANALYZER THE TA INSTRUMENTS DYNAMIC MECHANICAL ANALYZER The TA Instruments Q800 is the culmination of years of engineering expertise in Dynamic Mechanical Analyzers. TA
More information, to obtain a way to calculate stress from the energy function U(r).
BIOEN 36 013 LECTURE : MOLECULAR BASIS OF ELASTICITY Estimating Young s Modulus from Bond Energies and Structures First we consider solids, which include mostly nonbiological materials, such as metals,
More information8.2 Elastic Strain Energy
Section 8. 8. Elastic Strain Energy The strain energy stored in an elastic material upon deformation is calculated below for a number of different geometries and loading conditions. These expressions for
More informationEffect of Index on Curing Kinetics and Viscoelastic Properties of Polyurethane Gels
Effect of Index on Curing Kinetics and Viscoelastic Properties of Polyurethane Gels Lifeng Wu* and Rafael E. Camargo *Contact information: Lifeng Wu, Ph.D. Sr. Technical Specialist Huntsman Polyurethanes
More informationAdhesion and Viscoelasticity Properties of PVB in Laminated Safety Glass
Adhesion and Viscoelasticity Properties of PVB in Laminated Safety Glass Maurizio FROLI Professor Department of Civil Engineering, Structural Division University of Pisa, Pisa, Italy Maurizio Froli, born
More information2.5 Physicallybased Animation
2.5 Physicallybased Animation 320491: Advanced Graphics  Chapter 2 74 Physicallybased animation Morphing allowed us to animate between two known states. Typically, only one state of an object is known.
More informationQuestion 6.5: A steel bar 100 mm (4.0 in.) long and having a square cross section 20 mm
14:440:407 Ch6 Question 6.3: A specimen of aluminum having a rectangular cross section 10 mm 12.7 mm (0.4 in. 0.5 in.) is pulled in tension with 35,500 N (8000 lb f ) force, producing only elastic deformation.
More informationCHBE 363: Rotary Viscometer
CHBE 363: Rotary Viscometer Objectives 1. To illustrate the use of a rotary viscometer in the characterization of different types of fluids. 2. To determine the viscosity of Newtonian liquids. 3. To investigate
More informationMETU DEPARTMENT OF METALLURGICAL AND MATERIALS ENGINEERING
METU DEPARTMENT OF METALLURGICAL AND MATERIALS ENGINEERING Met E 206 MATERIALS LABORATORY EXPERIMENT 1 Prof. Dr. Rıza GÜRBÜZ Res. Assist. Gül ÇEVİK (Room: B306) INTRODUCTION TENSION TEST Mechanical testing
More informationDetermining the impact of electrical loss in coaxial cable
Determining the impact of electrical loss in coaxial cable Here's a discussion on cable attenuation based on the differences in dielectric loss of low density polyethylene resins and quantify the consequent
More informationFlow characteristics of microchannel melts during injection molding of microstructure medical components
Available online www.jocpr.com Journal of Chemical and Pharmaceutical Research, 2014, 6(5):112117 Research Article ISSN : 09757384 CODEN(USA) : JCPRC5 Flow characteristics of microchannel melts during
More informationAsphalt Specifications and Testing TriParty Transportation Conference Brett Lambden March 2324, 2015
Asphalt Specifications and Testing TriParty Transportation Conference Brett Lambden March 2324, 2015 Overview Asphalt Cement Production Composition Pavement Distresses Previous asphalt specifications
More informationMeasurement of Material Creep Parameters of Amorphous Selenium by Nanoindentation and the Relationship Between Indentation Creep and Uniaxial Creep
University of Tennessee, Knoxville Trace: Tennessee Research and Creative Exchange Masters Theses Graduate School 82004 Measurement of Material Creep Parameters of Amorphous Selenium by Nanoindentation
More informationDETERMINATION OF TIMETEMPERATURE SHIFT FACTOR FOR LONGTERM LIFE PREDICTION OF POLYMER COMPOSITES
DETERMINATION OF TIMETEMPERATURE SHIFT FACTOR FOR LONGTERM LIFE PREDICTION OF POLYMER COMPOSITES K. Fukushima*, H. Cai**, M. Nakada*** and Y. Miyano*** * Graduate School, Kanazawa Institute of Technology
More informationGlassy polymers and the nature of the glass transition. The factors that affect Tg
Thermal Transitions: Crystallization, Melting and the Glass Transition Today: Glassy polymers and the nature of the glass transition The factors that affect Tg Plasticizers Chapter 8 in CD (Polymer Science
More informationFluid Mechanics: Static s Kinematics Dynamics Fluid
Fluid Mechanics: Fluid mechanics may be defined as that branch of engineering science that deals with the behavior of fluid under the condition of rest and motion Fluid mechanics may be divided into three
More informationCBE 6333, R. Levicky 1 Review of Fluid Mechanics Terminology
CBE 6333, R. Levicky 1 Review of Fluid Mechanics Terminology The Continuum Hypothesis: We will regard macroscopic behavior of fluids as if the fluids are perfectly continuous in structure. In reality,
More informationRHEOLOGY RHEOLOGY Science describing the flow and deformation of matter under stress. Rheo = the flow Viscosity (η) is the resistance of a fluid material to flow under stress. The higher the viscosity,
More informationWhat is a mold? Casting. Die casting. Injection Molding Machine. Injection Molding. 2.008 Design & Manufacturing II. Spring 2004
2.008 Design & Manufacturing II What is a mold? From Webster: a cavity in which a substance is shaped: as (1) : a matrix for casting metal (2) : a form in which food is given a decorative shape Spring
More informationDE Actuated Automotive HVAC Louvers
DE Actuated Automotive HVAC Louvers Nick M Manzek Tizoc CruzGonzalez Jonathan Luntz GM/UM Smart Materials and Structures Collaborative Research Lab Diann Brei ABSTRACT Automotive manufacturers are always
More informationMechanical Properties  Stresses & Strains
Mechanical Properties  Stresses & Strains Types of Deformation : Elasic Plastic Anelastic Elastic deformation is defined as instantaneous recoverable deformation Hooke's law : For tensile loading, σ =
More informationFatigue :Failure under fluctuating / cyclic stress
Fatigue :Failure under fluctuating / cyclic stress Under fluctuating / cyclic stresses, failure can occur at loads considerably lower than tensile or yield strengths of material under a static load: Fatigue
More informationStatistical Mechanics, Kinetic Theory Ideal Gas. 8.01t Nov 22, 2004
Statistical Mechanics, Kinetic Theory Ideal Gas 8.01t Nov 22, 2004 Statistical Mechanics and Thermodynamics Thermodynamics Old & Fundamental Understanding of Heat (I.e. Steam) Engines Part of Physics Einstein
More informationGuide to the measurement of the flow properties of polymeric materials
Guide to the measurement of the flow properties of polymeric materials In processing plastics the material is melted, transferred and then solidified. The transfer or flow process is critical to processing
More informationKursus i Produktions og materialeteknologi
Kursus i Produktions og materialeteknologi Plastsprøjtestøbning / Injection Molding Basics Short history of plastics 1862 first synthetic plastic 1866 Celluloid 1891 Rayon 1907 Bakelite 1913 Cellophane
More informationUnderstanding Plastics Engineering Calculations
Natti S. Rao Nick R. Schott Understanding Plastics Engineering Calculations Handson Examples and Case Studies Sample Pages from Chapters 4 and 6 ISBNs 978569905098569905096 HANSER Hanser Publishers,
More informationME 612 Metal Forming and Theory of Plasticity. 3. Work Hardening Models
Metal Forming and Theory of Plasticity Yrd.Doç. e mail: azsenalp@gyte.edu.tr Makine Mühendisliği Bölümü Gebze Yüksek Teknoloji Enstitüsü In this section work hardening models that are applicable to different
More information1. Prereptation era and the birth of the tube model
Dynamics of Entangled Polymers Ideas Introduced by de Gennes and Others Outline 1. Prereptation era and the birth of the tube model 2. Reptation of linear polymers 3. Manychain effects constraint release
More information4 Microscopic dynamics
4 Microscopic dynamics In this section we will look at the first model that people came up with when they started to model polymers from the microscopic level. It s called the Oldroyd B model. We will
More informationModern Construction Materials Prof. Ravindra Gettu Department of Civil Engineering Indian Institute of Technology, Madras
Modern Construction Materials Prof. Ravindra Gettu Department of Civil Engineering Indian Institute of Technology, Madras Module  2 Lecture  3 Structure of Solids This is the third part of the lecture
More informationObjectives. Experimentally determine the yield strength, tensile strength, and modules of elasticity and ductility of given materials.
Lab 3 Tension Test Objectives Concepts Background Experimental Procedure Report Requirements Discussion Objectives Experimentally determine the yield strength, tensile strength, and modules of elasticity
More informationIntroduction to Instrumented Indentation Testing (IIT)
Introduction to Instrumented Indentation Testing (IIT) Innovation Center Oak Ridge, Tennessee Pierre Morel OUTLINE 1. Instrumented indentation testing Theory 2. MTS Instruments technology 3. Test knowledge
More informationCHAPTER 9 : MECHANICAL PROPERTIES OF SOLIDS ONE MARK QUESTIONS: 1. What is elasticity of a body? 2. What is plasticity? 3. Which property of a body
1 CHAPTER 9 : MECHANICAL PROPERTIES OF SOLIDS ONE MARK QUESTIONS: 1. What is elasticity of a body? 2. What is plasticity? 3. Which property of a body is responsible for regaining original shape and size
More informationMicroindentation characterization of polymers and polymer based nanocomposites. V. Lorenzo
Microindentation characterization of polymers and polymer based nanocomposites V. Lorenzo Hardness and hardness measurement Vickers hardness Relationships between hardness and other mechanical properties
More informationVISUAL PHYSICS School of Physics University of Sydney Australia. Why do cars need different oils in hot and cold countries?
VISUAL PHYSICS School of Physics University of Sydney Australia FLUID FLOW VISCOSITY POISEUILLE'S LAW? Why do cars need different oils in hot and cold countries? Why does the engine runs more freely as
More informationUnderstanding Rheology
Understanding Rheology Ross Clark Distinguished Research Fellow San Diego R&D Page 1 Background CP Kelco makes carbohydrate based water soluble polymers Fermentation Xanthan Gellan Plant derived Pectin
More informationDevelopments in Low Temperature Testing of Rubber Materials
Developments in Low Temperature Testing of Rubber Materials Technical report 01/4, 2nd edition Nov 2010 Göran Spetz Elastocon AB SWEDEN Introduction The low temperature properties of rubber materials are
More information(10 4 mm 2 )(1000 mm 3 ) = 10 7 mm = 10 4 m = 6.2 mi
CHAPTER 8 DEFORMATION AND STRENGTHENING MECHANISMS PROBLEM SOLUTIONS Basic Concepts of Dislocations Characteristics of Dislocations 8.1 To provide some perspective on the dimensions of atomic defects,
More informationStress and Deformation Analysis. Representing Stresses on a Stress Element. Representing Stresses on a Stress Element con t
Stress and Deformation Analysis Material in this lecture was taken from chapter 3 of Representing Stresses on a Stress Element One main goals of stress analysis is to determine the point within a loadcarrying
More informationExtrusion Simulation of Tire Components Using HyperXtrude
Extrusion Simulation of Tire Components Using HyperXtrude Vidit Bansal Dr. Jyoti Prakash Rath G. Unnikrishnan Tom Thomas Assistant Manager Head Vice President Executive Director Advanced Engineering(R&D)
More informationSolid Mechanics. Stress. What you ll learn: Motivation
Solid Mechanics Stress What you ll learn: What is stress? Why stress is important? What are normal and shear stresses? What is strain? Hooke s law (relationship between stress and strain) Stress strain
More informationPhase Change Module  ENGR 101
Notes for the Instructor Phase Change Module  ENGR 101 Lab 1: Demonstration: foam insulation in a can sprayed into a box. Shows how an aerosol propellant moves a liquid which transitions to a solid as
More informationDifferential Scanning Calorimetry theoretical background
Differential Scanning Calorimetry theoretical background Galina Kubyshkina Elektromaterial Lendava d.d., Slovenia Crystalline materials Typical features presence of a unit (cell), which is periodically
More informationThe Kinetic Theory of Gases Sections Covered in the Text: Chapter 18
The Kinetic Theory of Gases Sections Covered in the Text: Chapter 18 In Note 15 we reviewed macroscopic properties of matter, in particular, temperature and pressure. Here we see how the temperature and
More informationCh 2 Properties of Fluids  II. Ideal Fluids. Real Fluids. Viscosity (1) Viscosity (3) Viscosity (2)
Ch 2 Properties of Fluids  II Ideal Fluids 1 Prepared for CEE 3500 CEE Fluid Mechanics by Gilberto E. Urroz, August 2005 2 Ideal fluid: a fluid with no friction Also referred to as an inviscid (zero viscosity)
More informationTorsion Tests. Subjects of interest
Chapter 10 Torsion Tests Subjects of interest Introduction/Objectives Mechanical properties in torsion Torsional stresses for large plastic strains Type of torsion failures Torsion test vs.tension test
More informationI. INTRODUCTION: Phenomenology. N / m. N / m (2) kg G. Let s consider a shear force experiment on a solid cube. (Fig. 1)
I. INTRODUCTION: Phenomenology Let s consider a shear force experiment on a solid cube. (Fig. 1) We can easily verify that for the solid not to move or rotate, all forces acting on the cube must be of
More informationRheology of ParticleFoam Mixture
Aycan Özlem Özarmut Holger Steeb Rheologie Workshop 04. Juni 2014 TP Rheology of Foam 2 1 TP Foam in EPB Tunneling [Herrenknecht AG] Improvement of the fluidity and watertightness of excavated soil To
More informationStructural Axial, Shear and Bending Moments
Structural Axial, Shear and Bending Moments Positive Internal Forces Acting Recall from mechanics of materials that the internal forces P (generic axial), V (shear) and M (moment) represent resultants
More informationCourse in. Nonlinear FEM
Course in Introduction Outline Lecture 1 Introduction Lecture 2 Geometric nonlinearity Lecture 3 Material nonlinearity Lecture 4 Material nonlinearity continued Lecture 5 Geometric nonlinearity revisited
More informationSUPERPAVE PERFORMANCE GRADED BINDER TESTS. Superpave Performance Graded Binder Tests 1
SUPERPAVE PERFORMANCE GRADED BINDER TESTS Superpave Performance Graded Binder Tests 1 PG Specifications Fundamental properties related to pavement performance Environmental factors Inservice & construction
More informationMAE 20 Winter 2011 Assignment 5
MAE 20 Winter 2011 Assignment 5 6.7 For a bronze alloy, the stress at which plastic deformation begins is 275 MPa (40,000 psi), and the modulus of elasticity is 115 GPa (16.7 10 6 psi). (a) What is the
More informationPUMPS STEAM TURBINES BUILDING & FIRE WASTEWATER SERVICE PUMP CLINIC 22 VISCOSITY
PUMP CLINIC 22 VISCOSITY The viscosity of a fluid is that property which tends to resist a shearing force. It can be thought of as the internal friction resulting when one layer of fluid is made to move
More informationCh 8 Potential energy and Conservation of Energy. Question: 2, 3, 8, 9 Problems: 3, 9, 15, 21, 24, 25, 31, 32, 35, 41, 43, 47, 49, 53, 55, 63
Ch 8 Potential energ and Conservation of Energ Question: 2, 3, 8, 9 Problems: 3, 9, 15, 21, 24, 25, 31, 32, 35, 41, 43, 47, 49, 53, 55, 63 Potential energ Kinetic energ energ due to motion Potential energ
More informationChapter 12 Elasticity
If I have seen further than other men, it is because I stood on the shoulders of giants. Isaac Newton 12.1 The Atomic Nature of Elasticity Elasticity is that property of a body by which it experiences
More informationLinear Elastic Cable Model With Creep Proportional to Tension
610 N. Whitney Way, Suite 160 Madison, Wisconsin 53705, USA Phone No: (608) 2382171 Fax No: (608) 2389241 info@powline.com http://www.powline.com Linear Elastic Cable Model With Creep Proportional to
More informationStructural Integrity Analysis
Structural Integrity Analysis 1. STRESS CONCENTRATION Igor Kokcharov 1.1 STRESSES AND CONCENTRATORS 1.1.1 Stress An applied external force F causes inner forces in the carrying structure. Inner forces
More informationWhen the fluid velocity is zero, called the hydrostatic condition, the pressure variation is due only to the weight of the fluid.
Fluid Statics When the fluid velocity is zero, called the hydrostatic condition, the pressure variation is due only to the weight of the fluid. Consider a small wedge of fluid at rest of size Δx, Δz, Δs
More informationDeflections. Question: What are Structural Deflections?
Question: What are Structural Deflections? Answer: The deformations or movements of a structure and its components, such as beams and trusses, from their original positions. It is as important for the
More information